A study of the final stages of the austenite to martensite ... Transformation in SAE 1050 Steel
Embed Size (px)
Transcript of A study of the final stages of the austenite to martensite ... Transformation in SAE 1050 Steel
Journal of Research of the National Bureau of Standards Vol. 55, No.3, September 1955 Research Paper 2616
A Study of the Final Stages of the Austenite to Martensite Transformation in SAE 1050 Steel 1
Melvin R. Meyerson and Samuel J. Rosenberg
The austeni te-martens ite transformat ion curves in t he temperature range from M . to - 3200 F have been established for t wo SAE 1050 steels. No sign ifi cant effect of a usten it-iz ing temperature or austeni te grain size on the amount of martensite formed per degree d,'op in t ransformat ion temperat ure was observed at temperatures lower than about 1000 F below the M,. Wi t hin the limits t ested , cooling rate from the auste ni t izing temperature had no effect on t he austeni te-martensite t ransformation. The amount of martensite formed per degree drop in temperature decreased at transformation temperat ures of abou t 3500 F and below, and t he t ransformation did not go to completion eve n at the lowest temperature u tilized (- 320v F ). At t his temperature the amount of retained austeni te was about 1 percent.
The literature contains many references to investi-gations of the austenite-m.al'tensite reaction , par-ticularly the temperature at t he start of the trans-formation , the M s. Considerably fewer studies have been concerned wi th the completion of the martensite transformation , th e M t . Amon~ these are th e studies of Cohen  2, Averbach and Gohen , Averbach , Castleman , and Cohen , Roberts , Lyman and Troi ano , Harris and Cohen , Howard and Cohen , Grange and Stewart  , and Sadovski and Bogacheva  . In most of the work reported by these au thors, highly alloyed materials were used. Data on effects of such heat treating variables as austenitizing temperature and grain size on the M t of carbon steels are quite meager .
In a study  of the influence of austenitizing temperature, austenite grain size, and cooling rate on the mar tensite transforma tion in two SAE 1050 steels, the authors found that the M . was raised and that the ini tial quantities of martensite formed below the nrf. was decreased as the austenite grain size was increased. Austenitizing temperature had no effect on the 11. except insofar as it established the austen-ite grain size. Cooling rate, within the limits studied, also had no effect. This study has been extended to ascertain the effects of these h eat treating variables on the completion of the martensite transformation (M !) .
2 . Materials and Experimental Procedures
The same two steels that were used to study the effects of heat treating variables on the M s trans-formation were used for the presen t work. Their compositiqns, as given in table 1, were similar except that 11- 182 had a greater aluminum content and was of "controlled" grain size whereas 11- 179 was not.
The quen ch-temper method as described previ-ously  was used in this s tudy. As before, the
I This work was sponsored by Watertown Ar senal, Ordnance Corps, U . S. Army.
, Figures in brackets indicate tile literature refercnces at the end of this paper .
entire qu ench-temper cycle was limited to a maxi-mum time in terval of 11 sec in order to prevent the isothermal formation of bainite.
Specimens (0.050 in. X O.I0 in. X O.I0 in. ) were austenitized at 1,475 and 1,600 F for 7 min and at 1,750, 1,900, 2,025 , and 2,150 F for 3 min . The austenite grain sizes establish ed under these condi-tions are shown in table 2. Tho e specimens trans-formed above room temperature were quenched for 3 sec in 50 percent lead-50 pcrcen t b ismuth alloy and then tempered for 8 sec at 625 F in another pot containing the same alloy. The remainder were quenched to room temperature in water, to 19 F in iced brine, to - 105 F in a mixture of CCI4 + CHC13 + solid CO2, and to - 320 F in liquid nitro-gen. The approximate cooling rates of the small specimens in th ese media., as measUl'ed over the range 1,300 to 900 F were: Pb-Bi 5,000 F /sec, water 8,000 F /sec, iced brine 14,000 F /sec, CCI4+ CH CI3 + C0 2 320 F lsec, and liquid nitrogen 190 F Isec. Some of the specimens q llen ch ed directly to
TABLE 1. Chemical composition of the steels used P ercentagc by weight
S teel C Mn P S Si Ai2 IT 0 N 0 , Acid solu- Total ble
----- - - - - - ----- - - --M - 179 ___ _ 0.49 O. 79 0.023 0. 023
1. 22 0. 001 0.002 0. 0030. 00020.004 0. 004
1\1- 182. ___ 0. 491.80 0. 022
1. 2110' 007
1 0. 0161 0. 020
1 . 0002
T A BLE 2. Effect of austeniti zing conditions on grain size
Austen itizing AS'l'M grain size nu mber
'l'cmper~ 'rime M - li9 1\1- 182 ature ---- - - --- - - -
OF min 1, 475 7 8 8 1, 600 7 5 7- 8 1.750 3 4-5 5 1.900 3 4 5 2, 025 3 3 5 2, 150 3 2 3
-320 F in liquid nitrogen contained appreciable amounts of pearlite due to the slow cooling rate of the medium. This was particularly true of the fine-grained steel C~1-182) austenitized at 1,475 F. Therefore, some specimens were quenched to -320 F indirectly, with an intermediate quench of 6 sec in either iced brine or CC14+ CHCb + solid CO2 This procedure also afforded an opportunity to ob-serve any effect of the shor t delay in quenching on the M!; i. e., any stabilizing effect. Specimens quenched directly to - 320 F and which contained as much as one-half percent of pearlite were dis-carded.
An Einthoven string galvanometer, actuated by a thermocouple welded to the specimen, served to determine the temperature reached by the specimen just prior to tempering. This instrument was not used in conjunction with specimens quenched to room temperature or lower.
After mounting, all specimens were carefully ground to midpoint and given a metallographic pol-ish. Lineal analysis was employed to determine the amount of tempered martensite up to about 90 per-cent. When more than this was present, the light constituents (austenite plus fresh martensite) were too finely dispersed to permit accurate lineal analysis. Typical microstructures showing advanced stages of the austenite-martensite transformation are shown in figure 1. In order to determine the amount of austenite in specimens containing more than il bout 90 percent of martensite, X-ray diffraction tech-niques, similar to the integrated intensity method reported by Averbach and Cohen  were used. A modification in computil,tion described by Beu  was found to agree closely with the longer procedure of Averbach and Cohen and gave comparable results with less calculation. It was used throughout, with occasional verification by the longer method.
X-ray exposures were for 24 hr, using Co Ka radiation. A monochrometer equipped with a pent-aerythritol crystal was employed to reduce back-
ground; this crystal had a 20 angle of 23.60 when used with Co Ka radiation. Since X-ray methods could not be applied to specimens transformed at temperatures above ambient (subsequent cooling to room temperature would cause the transformation of some of the un transformed austenite) and since lineal analysis could not be used on specimens that had formed more than about 90 percent of martensite, no determinations could be made in this range (ap-proximately room temperature to about 350F). Consequently, all graphs of percent martensite versus transformation temperature plotted from experi-mental data have no points located in this range. The effect on the shape of the transformation curves (percent martensite versus transformation tempera-ture) was negligible, since the quantity of austenite transformed with decreasing temperatures was ex-tremely small both at temperatures just above and below this range.
A conventional powder camera of 57.3-mm diam was modified to accommodate the mounted speci-mens. The specimen holder was redesigned so as to allow the specimen to rotate slowly in the plane of its surface. By so doing the diffraction lines were uniformly free from spottiness except for specimens of steel M- 179 austenitized at 2,150F. The influ-ence of the large grains in this steel (ASTM No. 2) in causing spottiness could not be eliminated by rotation. Details of the modified camera are shown in figures 2 and 3. The amount of light transmitted through the austenite and martensite lines on the X-ray film was determined by means of a recording microphotometer. From these data the densi ty of the blackening curves was constructed on lineal scales and the areas under the peaks measured with a planimeter. The relative areas were used to compute the amounts of austenite and martensite. The film used was tested for linearity of blackening as a func-tion of the amount of exposure and was found to be linear in the ranges used .
FIGURE 1. Typical microstructures showing advanced stages oj the austenite-martensite transformation.
The martensite formed at the temperature of transformation has been darkened by snbsequent tempering; the light areas are fresh (un tempered) martensite plus retained austenite. Steel M- 182, etched with 1 percent nital plus 1 percent zephiran chloride. X750.
a, Transformed at 5100 F, 62% martenSite; b, t ransformed at 4650 F, 81% marteusite; c, transfo rmed a t 4100 F , 93% martensite. Quantitative determinct tions by lineal analysis of structures of th is type are difficult. It represents the approximate limit for which lineal analYSis was used .
FIGURE 2. lYlodijied X-my camem, assembled view with cover removed.
X approx. }2.
3 . Results
The amount of martensite formed upon quenching to different temperature levels below M . and down to - 310 F was determined experimentally and then plotted to obtain transformation curves similar to the typical curves shown in figure 4. A complete curve, a